Physical and mechanical properties of western juniper have been examined and markets for a wide variety of juniper products have been explored. Examples of products that have been explored include: cement/woodfiber composites, particleboard, hardboard, animal bedding (shavings), fencing, decking, interior doors, paneling, flooring, veneer, furniture, and novelty items.
Researchers at the USDA Forest Products Laboratory in Madison, WI, have characterized the fiber properties and chemistry of western juniper and summarized the results in the report: Basic Fiber and Chemical Properties of Western Juniper.
Western juniper heartwood is highly durable (similar to redwood and cedars) and has aromatic properties like its close relative eastern redcedar (Juniperus virginiana). The color of the wood varies from milky white to deep reddish-brown and has large, swirling grain patterns and bands of heartwood mixed with sapwood, similar to eastern redcedar. Tests have shown juniper wood to machine, glue, and finish well. Once dried, juniper wood shrinks and swells less than many other Pacific Northwest species such as Douglas-fir, ponderosa pine, and western redcedar. Juniper has some unique bending properties. After being soaked in hot water, thin (1/32"-1/16") samples have been tied into intricate knots without splitting.
Juniper wood is slightly more dense than ponderosa pine. The wood is also quite hard for a softwood: about 35% harder than ponderosa pine, but only about ½ as hard as red oak. Juniper is about 70% as stiff as ponderosa pine, and 85% as stiff as incense-cedar, meaning the wood deforms relatively easily under loads. The table below compares some of the mechanical and physical properties of western juniper with other commonly used woods.
Mechanical and Physical Properties of Western Juniper and Other Commonly Used Woods
|Species||Specific Gravity @12% MC||Density (lbs/ft3) @12% MC||Compression Strength-parallel to grain @12% MC (psi)||MOE- Bending Stiffness @12% MC (Million psi)||MOR-Bending Strength @12% MC (psi)|
|northern red oak||0.63||44||6760||1.82||14300|
|Species||Hardness @12% MC (lbs.)||Volumetric Shrinkage (%)||Nail Withdrawal Strength (side grain) (psi)||Machining||Gluing||Finishing||Bending|
|northern red oak||1290||13.7||363||VG||F||F||E|
Specific Gravity- Similar to density. Calculated as the weight of a sample of wood (oven dry) divided by the weight of an equal volume of water. In this
instance, the wood's volume was measured when the wood was at 12% moisture content. Another way to look at specific gravity is- If a wood species has a
specific gravity of 0.44, then the wood is 44% as heavy as water.
Density- Density of the wood in lbs. per cubic foot at 12% moisture content.
Compression Strength- Answers the question, "How strong is the wood when used as a column, such as a wall stud?". Determined by loading a wood sample
as a column and recording the stress (psi) at the proportional limit. The proportional limit is a point on a graph of deformation versus load. The proportional
limit is the point at which there is no longer a straight-line relationship between load (lbs.) and the amount the wood column deforms in inches. A low
compression strength indicates the wood may crush fairly easily if used as a support column.
Bending Stiffness- Answers the question, "How stiff is the wood when bent like a floor joist?". Determined by loading a wood sample as a beam and
recording the stress (psi) at the proportional limit. (see discussion of compression strength above for a description of proportional limit). A low stiffness
value indicates the wood may be "spongy" or "springy" if not adequately supported in decking. Long, unsupported spans would be unwise for floor joists.
Bending Strength- Answers the question, "How strong is the wood when bent like a floor joist?". Similar to bending stiffness, except the wood beam is
loaded until it breaks. Note the distinction between stiffness and strength. Stiffness is how easily the wood bends, strength is how much force it takes to
break the sample.
Hardness- Answers the question, "How resistant is the wood to wear and marring, such as when used for flooring?". Hardness is measured by recording the
amount of force it takes to embed a 0.444 inch diameter ball to half its diameter into the wood. A low hardness value means the wood would dent easily if
used in flooring.
Volumetric Shrinkage- Answers the question, "How stable is the wood?". Table values are percent shrinkage from green to ovendry. This value is useful for
comparisons to other species. As an example, a ponderosa pine board will shrink, on the average, 9.7% in total volume from green to oven dry. Western
juniper will only shrink 82% as much as ponderosa pine. Actual inches of shrinkage in the radial and the tangential direction may be calculated using
published shrinkage coefficients.
Nail Withdrawal Strength- Answers the question, "How well does the wood hold a nail?". Measured as the amount of force required to pull a nail from the
wood. A low nail withdrawal value would indicate that nails may pop up easily if the wood shrinks or swells or that nailed joints may be excessively weak.
Table values for species other than western juniper are estimated using a formula from the USDA's Wood Handbook.
The last 4 properties (machining, gluing, finishing, and bending) in the table are subjective. The table lists those properties as: E (excellent), VG (very
good), G (good), F (fair), or P (poor).
Machining- How well does the wood machine? Does the wood tend to burn or chip during cutting, surfacing, and moulding operations?
Gluing- Does the wood glue well? Do chemical extractives in the wood prevent the formation of strong bonds?
Finishing- How easy is it to keep a finish on the surface?
Bending- How well does the wood bend? Does the wood split during bending?
Values for western juniper from Dr. Ed Burke, School of Forestry, University of Montana. Other values are from the Wood Handbook: Wood as
an Engineering Material, USDA Forest Service, Forest Products Laboratory, Ag. Handbook #72, 1987.
top of page